Series of chiral interpenetrating 3d‒4f heterometallic MOFs: Luminescent sensors and magnetic properties
Zhang, Xiaolei; Chen, Chen; Liu, Xiaoli; Gao, Peng; Hu, Ming; Journal of Solid State Chemistry 253 (2017) 360–366; doi:10.1016/j.jssc.2017.06.020

data_1560412
_publ_section_title
;
 Series of chiral interpenetrating 3d--4f heterometallic MOFs: Luminescent
 sensors and magnetic properties
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              360
_journal_page_last               366
_journal_paper_doi               10.1016/j.jssc.2017.06.020
_journal_volume                  253
_journal_year                    2017
_chemical_formula_sum            'C24 H16 Eu N3 O9 Zn'
_chemical_formula_weight         707.76
_space_group_IT_number           78
_space_group_name_Hall           'P 4cw'
_space_group_name_H-M_alt        'P 43'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'P 43'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.2456(6)
_cell_length_b                   12.2456(6)
_cell_length_c                   15.2080(11)
_cell_measurement_temperature    293(2)
_cell_volume                     2280.5(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0928
_diffrn_reflns_av_sigmaI/netI    0.0955
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            14957
_diffrn_reflns_theta_full        67.23
_diffrn_reflns_theta_max         67.23
_diffrn_reflns_theta_min         3.61
_exptl_absorpt_coefficient_mu    21.348
_exptl_absorpt_correction_T_max  0.224
_exptl_absorpt_correction_T_min  0.226
_exptl_crystal_colour            yello
_exptl_crystal_density_diffrn    2.061
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1384
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.07
_refine_diff_density_max         1.419
_refine_diff_density_min         -0.756
_refine_diff_density_rms         0.153
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.026(7)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.027
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     349
_refine_ls_number_reflns         4057
_refine_ls_number_restraints     1111
_refine_ls_restrained_S_all      0.922
_refine_ls_R_factor_all          0.0912
_refine_ls_R_factor_gt           0.0695
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0911P)^2^+7.2972P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1658
_refine_ls_wR_factor_ref         0.1784
_reflns_number_gt                3177
_reflns_number_total             4098
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2017-253-360.cif
_cod_data_source_block           exp_6101
_cod_original_sg_symbol_H-M      P43
_cod_database_code               1560412